Page:EB1911 - Volume 16.djvu/362

Rh The “single-bath process” consists of paddling, drumming, or otherwise introducing into the skins a solution of a chrome salt, usually chrome alum, which is already in the basic condition, and therefore does not require reducing. The basic solutions are made as follows: For 100 ℔ of pelts 9 ℔ of chrome alum are dissolved in 9 gallons of water, and 2 ℔ of washing soda already dissolved in 1 gallon of water are gradually added, with constant stirring. One-third of the solution is added to 80 gallons of water, to which is added 7 ℔ of salt, and the skins are introduced; the other two-thirds are introduced at intervals in two successive portions. Another liquor, used in the same way, is made by dissolving 3 ℔ of potassium bichromate in hot water, adding gallon strong hydrochloric acid and then, gradually, about 1 ℔ of glucose or grape sugar; this reduces the acidic chrome salt, vigorous effervescence ensuing. The whole is made up to 2 gallons and 5% to 15% of salt is added. In yet another method a chrome alum solution is rendered basic by boiling with “hypo,” and after the reaction has ceased the solution is allowed to settle and the clear portion used.

After tanning, which takes from 8 hours to as many, and even more, days, depending upon the method used and the class of skin being dressed, the skins tanned by both methods are treated in a similar manner, and are neutralized by drumming in borax solution, when they are washed free from borax by drumming in warm water, and are ready for dyeing, a process which will be dealt with further on. The goods are sometimes tanned by suspension, but this method is generally reserved for the tanning of the heavier leathers, which are treated in much the same way, the several processes taking longer.

Iron Tannage.—Before leaving mineral tanning, mention may be made of iron tannage, although this has gained no prominent position in commerce. Ferric salts possess powerful tanning properties, and were thoroughly investigated by Professor Knapp, who took out several patents, but the tendency to produce a brittle leather has never been entirely overcome, although it has been greatly modified by the incorporation of organic matter, such as blood, rosin, paraffin, urine, &c. Knapp’s basic tanning liquor is made as follows: A strong solution of ferrous sulphate is boiled and then oxidized to the ferric state by the careful addition of nitric acid. Next, to destroy excess of nitric acid, ferrous sulphate is added until effervescence ceases and the resulting clear orange-coloured solution is concentrated to a varnish-like consistency. It does not crystallize or decompose on concentration. The hides or skins are prepared for tanning in the usual way, and then handled or otherwise worked in solutions of the above iron salt, the solutions, which are at first weak, being gradually strengthened.

The tannage occupies from 2 to 8 days, and the goods are then stuffed in a ventilated drum with greases or soap. If the latter is used, an insoluble iron soap is precipitated on the fibres of the leather, which may then be finally impregnated with stearin and paraffin, and finished in the usual manner as described under Curried Leathers. A very fair leather may also be manufactured by using iron alum and salt in the same manner as described under ordinary alum and salt.

Combination Tannages.—Leathers tanned by mixtures or separate baths of both mineral and vegetable tanning agents have now taken an important position in commerce. Such leathers are the Swedish and Danish glove leathers, the United States “dongola leather,” and French glazed kid. The usefulness of such a combination will be evident, for while vegetable tanning produces fullness, plumpness and resistance to water, the mineral dressing produces a softness unnatural to vegetable tannages without the use of large quantities of oils and fats. It may also be noted that once a leather has been thoroughly tanned with either mineral or vegetable materials, although it will absorb large quantities of the material which has not been first used, it will retain in the main the characteristics of the tannage first applied. The principle had long been used in the manufacture of such tough and flexible leathers as “green leather,” “combing leather” and “picker bands,” but was first applied to the manufacture of imitation glazed kid by Kent in America, who, about 1878, discovered the principle of “fatliquoring,” and named his product “dongola leather.” The discovery of this process revolutionized the manufacture of combination leathers.

The Swedish and Danish glove leathers were first given a dressing of alum and salt, with or without the addition of flour and egg, and were then finished and coloured with vegetable materials, generally with willow bark, although, in cases of scarcity, sumach, oak bark, madder and larch were resorted to. The “green leathers” manufactured in England generally receive about a week’s tannage in gambier liquors, and are finished off in hot alum and salt liquors, after which they are dried, have the crystallized salts slicked off, are damped back, and heavily stuffed with moellon, degras or sod oil. Kent, in the manufacture of his dongola leather, used mixed liquors of gambier alum and salt, and when tanned, washed the goods in warm water to remove excess of tanning agent, piled up to samm, and fatliquored. In making alum combinations it must be borne in mind that alum leather will not glaze, and if a glazed finish is required, a fairly heavy vegetable tannage should be first applied. For dull finishes the mineral tannage may advantageously precede the vegetable.

Very excellent chrome combination leather is also manufactured by the application of the above principles, gambier always being in great favour as the vegetable agent. The use of other materials deprives the leather of its stretch, although they may be advantageously used where the latter property is objectionable.

Oil Tanning.—Under the head of oil tanning is included “buff leather,” “buck leather,” “piano leather,” “chamois leather,” and to a greater or lesser extent, “Preller’s crown or helvetia leather.” The process of oil tanning dates back to antiquity, and was known as “shamoying,” now spelt “chamoising.” Chamoising yields an exceedingly tough, strong and durable leather, and forms an important branch of the leather industry. The theory of the process is the same as the theory of currying, which is nothing more or less than chamoising, viz. the lubrication of the fibres by the oil itself and the aldehyde tanning which takes place, due to the oxidation and decomposition of the esters of the fatty acids contained in the oil. The fact that an aldehyde tannage takes place seems to have been first discovered by Payne and Pullman, who took out a patent in 1898, covering formaldehyde and other aldehydes used in alkaline solutions. Their product, “Kaspine” leather, found considerable application in the way of military accoutrements. Chamois, buff, buck and piano leathers are all manufactured by the same process slightly modified to suit the class of hide used, the last three being heavy leathers, the first light.

As regards the process used for chamois leather, the reader will remember, from the account of the vegetable tannage of sheep skins, that after splitting from the limes, the fleshes were thrown back into the pits for another three weeks’ liming (six weeks in all) preparatory to being dressed as chamois leather. It is necessary to lime the goods for oil dressing very thoroughly, and if the grain has not been removed by splitting, as in the case of sheep skins, it is “frized” off with a sharp knife over the beam. The goods are now rinsed, scudded and drenched, dried out until stiff, and stocked in the faller stocks with plenty of cod oil for 2 to 3 hours until they show signs of heating, when they are hung up in a cool shed. This process is repeated several times during a period of from 4 to 6 days, the heat driving the water out of the skins and the oil replacing it. At the end of this time the goods, which will have changed to a brown colour, are hung up and allowed to become as dry as possible, when they are hung in a warm stove for some hours, after which they are piled to heat off, thrown into tepid water and put through a wringing machine. The grease which is recovered from the wringing machine is known commercially as “degras” or “moellon,” and fetches a good price, as it is unrivalled for fatliquoring and related processes, such as stuffing, producing a very soft product. They next receive a warm soda lye bath, and are again wrung; this removes more grease, which forms soap with the lye, and is recovered by treatment with vitriol, which decomposes the soap. The grease which floats on top of the liquor is sold under the name of “sod oil.” This also is a valuable material for fatliquoring, &c., but not so good as degras.

After being wrung out, the goods are bleached by one of the processes mentioned in the section on wool rug dressing, the permanganate method being in general use in England. In countries where a fine climate prevails the soap bleach or “sun bleach” is adopted; this consists of dipping the goods in soap solution and exposing them to the sun’s rays, the process being repeated three or more times as necessary.

The next step is fatliquoring to induce softness, after which they are dried out slowly, staked or “perched” with a moon knife, fluffed on a revolving wheel covered with fine emery to produce the fine “nap” or surface, brushed over with french chalk, fuller’s earth or china clay, and finally finished on a very fine emery wheel.

Preller’s Helvetia or Crown Leather.—This process of leather manufacture was discovered in 1850 by Theodor Klemm, a cabinetmaker of Württemberg, who being then in poor circumstances, sold his patent to an Englishman named Preller, who manufactured it in Southwark, and adopted a crown as his trade mark. Hence the name “crown” leather. The manufacture then spread through Switzerland and Germany, the product being used in the main for picker straps, belting and purposes where waterproof goods were required, such as hose pipes and military water bags. No taste is imparted to the water by this leather.